SSPC-SP 6 Surface Preparation Speciﬁcation No. 68
3. Ordering Information
3.1 The inclusion of the following, as required will describe
the desired material adequately, when ordered under this
3.1.1 Quantity (feet or number of lengths),
3.1.2 Name of material (seamless carbon steel pipe),
3.1.3 Grade (Table 1),
3.1.4 Manufacture (hot-ﬁnished or cold-drawn),
3.1.5 Size (NPS and weight class or schedule number, or
both; outside diameter and nominal wall thickness; or inside
diameter and nominal wall thickness),
3.1.6 Special outside diameter tolerance pipe (16.2.2),
3.1.7 Inside diameter tolerance pipe, over 10 in. (254 mm)
3.1.8 Length (speciﬁc or random, Section 20),
3.1.9 Optional requirements (Section 9 and S1 to S7),
3.1.10 Test report required (Section on Certiﬁcation of
Speciﬁcation A 530/A 530M),
3.1.11 Speciﬁcation designation,
3.1.12 End use of material,
3.1.13 Hydrostatic test in accordance with Speciﬁcation
A 530/A 530M or 13.3 of this speciﬁcation, or NDE in
accordance with Section 14 of this speciﬁcation.
3.1.14 Special requirements.
4.1 The steel shall be killed steel, with the primary melting
process being open-hearth, basic-oxygen, or electric-furnace,
possibly combined with separate degassing or reﬁning. If
secondary melting, using electroslag remelting or vacuum-arc
remelting is subsequently employed, the heat shall be deﬁned
as all of the ingots remelted from a single primary heat.
4.2 Steel cast in ingots or strand cast is permissible. When
steels of different grades are sequentially strand cast, identiﬁ-
cation of the resultant transition material is required. The
producer shall remove the transition material by any estab-
lished procedure that positively separates the grades.
4.3 For pipe NPS 11⁄2 and under, it shall be permissible to
furnish hot ﬁnished or cold drawn.
4.4 Unless otherwise speciﬁed, pipe NPS 2 and over shall be
furnished hot ﬁnished. When agreed upon between the manu-
facturer and the purchaser, it is permissible to furnish cold-
5. Heat Treatment
5.1 Hot-ﬁnished pipe need not be heat treated. Cold-drawn
pipe shall be heat treated after the ﬁnal cold draw pass at a
temperature of 1200°F (650°C) or higher.
6. General Requirements
6.1 Material furnished to this speciﬁcation shall conform to
the applicable requirements of the current edition of Speciﬁ-
cation A 530/A 530M unless otherwise provided herein.
7. Chemical Composition
7.1 The steel shall conform to the requirements as to
chemical composition prescribed in Table 1.
8. Heat Analysis
8.1 An analysis of each heat of steel shall be made by the
steel manufacturer to determine the percentages of the ele-
ments speciﬁed in Section 7. If the secondary melting pro-
cesses of 5.1 are employed, the heat analysis shall be obtained
from one remelted ingot or the product of one remelted ingot
of each primary melt. The chemical composition thus deter-
mined, or that determined from a product analysis made by the
manufacturer, if the latter has not manufactured the steel, shall
be reported to the purchaser or the purchaser’s representative,
and shall conform to the requirements speciﬁed in Section 7.
9. Product Analysis
9.1 At the request of the purchaser, analyses of two pipes
from each lot (Note 4) of 400 lengths or fraction thereof, of
each size up to, but not including, NPS 6, and from each lot of
200 lengths or fraction thereof of each size NPS 6 and over,
shall be made by the manufacturer from the ﬁnished pipe. The
results of these analyses shall be reported to the purchaser or
the purchaser’s representative and shall conform to the require-
ments speciﬁed in Section 7.
9.2 If the analysis of one of the tests speciﬁed in 9.1 does
not conform to the requirements speciﬁed in Section 7,
analyses shall be made on additional pipes of double the
original number from the same lot, each of which shall
conform to requirements speciﬁed.
NOTE 4—A lot shall consist of the number of lengths speciﬁed in
Sections 9 and 21 of the same size and wall thickness from any one heat
10. Tensile Requirements
10.1 The material shall conform to the requirements as to
tensile properties prescribed in Table 2. Computed elongation
values are contained in Table 3 and Table 4.
Available from Steel Structures Painting Council, 4400 5th Ave., Pittsburgh, PA
TABLE 1 Chemical Requirements
Grade A Grade B Grade C
0.25 0.30 0.35
Manganese 0.27–0.93 0.29–1.06 0.29–1.06
Phosphorus, max 0.035 0.035 0.035
Sulfur, max 0.035 0.035 0.035
Silicon, min 0.10 0.10 0.10
0.40 0.40 0.40
0.40 0.40 0.40
0.15 0.15 0.15
0.40 0.40 0.40
0.08 0.08 0.08
For each reduction of 0.01 % below the speciﬁed carbon maximum, an
increase of 0.06 % manganese above the speciﬁed maximum will be permitted up
to a maximum of 1.35 %.
These ﬁve elements combined shall not exceed 1 %.
TABLE 4 Elongation Values
Tension Test Specimen Wall Thickness, in.B
Elongation in 2 in. min., Speciﬁed Tensile Strength, psi
Grade A Grade B
1⁄2 in. Specimen 3⁄4 in. Specimen 1 in. Specimen 1 1⁄2 in. Specimen 48 000 60 000 70 000
$ 0.75 $ 1.491 $ 0.994 $ 0.746 $ 0.497 36.0 29.5 25.5
0.74 1.470–1.490 0.980–0.993 0.735–0.745 0.490–0.496 36.0 29.5 25.5
0.73 1.451–1.469 0.967–0.979 0.726–0.734 0.484–0.489 36.0 29.5 25.5
0.72 1.430–1.450 0.954–0.966 0.715–0.725 0.477–0.483 36.0 29.5 25.5
0.71 1.411–1.429 0.941–0.953 0.706–0.714 0.471–0.476 35.5 29.0 25.5
0.70 1.390–1.410 0.927–0.940 0.695–0.705 0.464–0.470 35.5 29.0 25.5
0.69 1.371–1.389 0.914–0.926 0.686–0.694 0.457–0.463 35.5 29.0 25.5
0.68 1.350–1.370 0.900–0.913 0.675–0.685 0.450–0.456 35.5 29.0 25.0
0.67 1.331–1.349 0.887–0.899 0.666–0.674 0.444–0.449 35.5 29.0 25.0
0.66 1.310–1.330 0.874–0.886 0.655–0.665 0.437–0.443 35.0 29.0 25.0
0.65 1.291–1.309 0.861–0.873 0.646–0.654 0.431–0.436 35.0 28.5 25.0
0.64 1.270–1.290 0.847–0.860 0.635–0.645 0.424–0.430 35.0 28.5 25.0
0.63 1.251–1.269 0.834–0.846 0.626–0.634 0.417–0.423 35.0 28.5 25.0
0.62 1.230–1.250 0.820–0.833 0.615–0.625 0.410–0.416 35.0 28.5 25.0
0.61 1.211–1.229 0.807–0.819 0.606–0.614 0.404–0.409 34.5 28.5 24.5
TABLE 2 Tensile Requirements
Grade B Grade C
Tensile strength, min, psi (MPa)
Yield strength, min, psi (MPa)
48 000 (330)
30 000 (205)
60 000 (415)
35 000 (240)
70 000 (485)
40 000 (275)
Elongation in 2 in. or 50 mm, min, %:
Basic minimum elongation transverse strip tests, and for all small
sizes tested in full section
35 25 30 16.5 30 16.5
When standard round 2-in. or 50-mm gage length test specimen is
28 20 22 12 20 12
For longitudinal strip tests A,B A,B A,B
For transverse strip tests, a deduction for each1⁄32-in. (0.8-mm)
decrease in wall thickness below 5⁄16in. (7.9 mm) from the basic
minimum elongation of the following percentage shall be made
The minimum elogation in 2 in. (50.8 mm) shall be determined by the following equation:
e 5 625 000A0.2
/ U 0.9
e = minimum elongation in 2 in. (50.8 mm), %, rounded to the nearest 0.5%
A = cross-sectional area of the tension test specimen, in.2
, based on speciﬁed outside diameter or nominal specimen width and speciﬁed wall thickness rounded to
the nearest 0.01 in. 2
(if the area thus caluclated is greater than the value 0.75 in. 2
shall be used), and
U = speciﬁed tensile strength, psi.
See Table number 4 for minimum elongation values for various size tension specimens and grades.
Table number 3 gives the computed minimum values:
TABLE 3 Computed Transverse ElongationA
Wall Thickness Elongation in 2 in. or 50 mm, min, %
in. mm Grade A, Transverse Grades B and C, Transverse
5⁄16 (0.312) 7.9 25.00 16.50
9⁄32 (0.281) 7.1 23.75 15.50
1⁄4(0.250) 6.4 22.50 14.50
This table gives the computed minimum elongation values for each 1⁄32-in. (0.8-mm) decrease in wall thickness. Where the wall thickness lies between two values
shown above, the minimum elongation value is determined by the following equation:
Grade Direction of Test Equation
B and C
E = 40t + 12.50
E = 32t + 6.50
E = elongation in 2 in. or 50 mm, %, and
t = actual thickness of specimen, in.
outside diameter (as shown in ANSI B 36.10) of the pipe,
11.2 Subject to the approval of the purchaser, for pipe
whose diameter exceeds 10 in. (254 mm), it shall be permis-
sible for the bend test to be substituted for the ﬂattening test
described in Section 12. The bend test specimens shall be bent
at room temperature through 180° with the inside diameter of
the bend being 1 in. (25.4 mm), without cracking on the outside
portion of the bent portion.
11.3 For pipe whose diameter exceeds 25 in. (635 mm) and
whose diameter to wall thickness ratio is 7.0 or less, the bend
test described in 11.2 shall be conducted instead of the
NOTE 5—Diameter to wall thickness ratio = speciﬁed outside diameter/
nominal wall thickness.
Example: For 28 in. diameter 5.000 in. thick pipe the diameter to wall
thickness ratio = 28/5 = 5.6.
12. Flattening Tests
12.1 Except as allowed by 11.2, for pipe over NPS 2, a
section of pipe not less than 21⁄2 in. (63.5 mm) in length shall
be ﬂattened cold between parallel plates until the opposite
walls of the pipe meet. Flattening tests shall be in accordance
with Speciﬁcation A 530/A 530M, except that in the formula
used to calculate the “H” value, the following “e” constants
shall be used:
0.08 for Grade A
0.07 for Grades B and C
12.2 When low D-to-t ratio tubulars are tested, because the
strain imposed due to geometry is unreasonably high on the
inside surface at the six and twelve o’clock locations, cracks at
these locations shall not be cause for rejection if the D-to-t ratio
is less than ten.
NOTE 6—The H values have been calculated for sizes from NPS 21⁄2 to
24, inclusive, and are shown in Table X1.1 of this speciﬁcation.
13. Hydrostatic Test
13.1 Each length of pipe shall withstand without leakage
through the pipe wall, a hydrostatic test, except as provided for
in 13.2, 13.3, and 13.4.
13.2 When speciﬁed by the purchaser, it shall be permis-
sible for pipe to be tested by the nondestructive electric test
described in Section 14 in lieu of the hydrostatic test.
13.3 When speciﬁed in the order, pipe shall be furnished
without hydrostatic test and without the NDE in Section 14. In
this case, each length so furnished shall include the mandatory
marking of the letters “NH.”
13.4 When the hydrostatic test and the NDE test are omitted
and the lengths marked with the letters “NH,” the certiﬁcation,
when required, shall clearly state “Not Hydro Statically
Tested,” the speciﬁcation number and material grade, as shown
on the certiﬁcation, shall be followed by the letters “NH.”
14. Nondestructive Electric Test
14.1 When allowed by 13.2, each pipe shall be tested with
a nondestructive electric test in accordance with Practice
E 213, Practice E 309, or Practice E 570. In such cases, the
marking of each length of pipe so furnished shall include the
letters “NDE.” It is the intent of this test to reject pipe with
imperfections that produce test signals equal or greater than
that of the calibration standard.
14.2 When the nondestructive electric test is performed, the
lengths shall be marked with the letters “NDE.” The certiﬁca-
tion, when required, shall state “Nondestructive Electric
Tested” and shall indicate which of the tests was applied. Also
the letters “NDE” shall be appended to the product speciﬁca-
tion number and material grade shown on the certiﬁcation.
14.3 The following information is for the beneﬁt of the user
of this speciﬁcation:
14.3.1 The reference standards deﬁned in 14.4 through 14.6
are convenient standards for calibration of nondestructive
testing equipment. The dimensions of such standards are not to
be construed as the minimum sizes of imperfections detectable
by such equipment.
14.3.2 The ultrasonic testing referred to in this speciﬁcation
is capable of detecting the presence and location of signiﬁcant
longitudinally or circumferentially oriented imperfections:
however, different techniques need to be employed for the
detection of such differently oriented imperfections. Ultrasonic
testing is not necessarily capable of detecting short, deep
14.3.3 The eddy current examination referenced in this
speciﬁcation has the capability of detecting signiﬁcant imper-
fections, especially of the short abrupt type.
14.3.4 The ﬂux leakage examination referred to in this
speciﬁcation is capable of detecting the presence and location
of signiﬁcant longitudinally or transversely oriented imperfec-
tions: however, different techniques need to be employed for
the detection of such differently oriented imperfections.
14.3.5 The hydrostatic test referred to in Section 13 has the
capability of ﬁnding defects of a size permitting the test ﬂuid
to leak through the tube wall and may be either visually seen
or detected by a loss of pressure. Hydrostatic testing is not
necessarily capable of detecting very tight, through-the-wall
imperfections or imperfections that extend an appreciable
distance into the wall without complete penetration.
14.3.6 A purchaser interested in ascertaining the nature
(type, size, location, and orientation) of discontinuities that can
be detected in the speciﬁc applications of these examinations is
directed to discuss this with the manufacturer of the tubular
14.4 For ultrasonic testing, the calibration reference notches
shall be, at the option of the producer, any one of the three
common notch shapes shown in Practice E 213. The depth of
notch shall not exceed 121⁄2 % of the speciﬁed wall thickness of
the pipe or 0.004 in. (0.102 mm), whichever is greater.
14.5 For eddy current testing, the calibration pipe shall
contain, at the option of the producer, any one of the following
discontinuities to establish a minimum sensitivity level for
14.5.1 Drilled Hole—The calibration pipe shall contain
depending upon the pipe diameter three holes spaced 120°
apart or four holes spaced 90° apart and sufficiently separated
longitudinally to ensure separately distinguishable responses.
The holes shall be drilled radially and completely through the
pipe wall, care being taken to avoid distortion of the pipe while
drilling. Depending upon the pipe diameter the calibration pipe
shall contain the following hole:
#1⁄2 in. 0.039 in. (1 mm)
>1⁄2 # 11⁄4 in. 0.055 in. (1.4 mm)
>11⁄4 # 2 in. 0.071 in. (1.8 mm)
>2 # 5 in. 0.087 in. (2.2 mm)
>5 in. 0.106 in. (2.7 mm)
14.5.2 Transverse Tangential Notch—Using a round tool or
ﬁle with a 1⁄4in. (6.4-mm) diameter, a notch shall be ﬁled or
milled tangential to the surface and transverse to the longitu-
dinal axis of the pipe. Said notch shall have a depth not
exceeding 121⁄2 % of the speciﬁed wall thickness of the pipe or
0.004 in. (0.102 mm), whichever is greater.
14.5.3 Longitudinal Notch—A notch 0.031 in. (0.787 mm)
or less in width shall be machined in a radial plane parallel to
the tube axis on the outside surface of the pipe, to have a depth
not exceeding 121⁄2 % of the speciﬁed wall thickness of the
tube or 0.004 in. (0.102 mm), whichever is greater. The length
of the notch shall be compatible with the testing method.
14.5.4 Compatibility—The discontinuity in the calibration
pipe shall be compatible with the testing equipment and the
method being used.
14.6 For ﬂux leakage testing, the longitudinal calibration
reference notches shall be straight-sided notches machined in a
radial plane parallel to the pipe axis. For wall thickness under
1⁄2 in. (12.7 mm), outside and inside notches shall be used; for
wall thickness equal and above 1⁄2 in. (12.7 mm), only an
outside notch shall be used. Notch depth shall not exceed
121⁄2 % of the speciﬁed wall thickness, or 0.004 in. (0.102
mm), whichever is greater. Notch length shall not exceed 1 in.
(25.4 mm), and the width shall not exceed the depth. Outside
diameter and inside diameter notches shall be located suffi-
ciently apart to allow separation and identiﬁcation of the
14.7 Pipe containing one or more imperfections that pro-
duce a signal equal to or greater than the signal produced by the
calibration standard shall be rejected or the area producing the
signal shall be reexamined.
14.7.1 Test signals produced by imperfections which cannot
be identiﬁed, or produced by cracks or crack-like imperfections
shall result in rejection of the pipe, unless it is repaired and
retested. To be accepted, the pipe must pass the same speciﬁ-
cation test to which it was originally subjected, provided that
the remaining wall thickness is not decreased below that
permitted by this speciﬁcation. The OD at the point of grinding
may be reduced by the amount so reduced.
14.7.2 Test signals produced by visual imperfections such as
those listed below may be evaluated in accordance with the
provisions of Section 18:
18.104.22.168 Straightener marks,
22.214.171.124 Cutting chips,
126.96.36.199 Steel die stamps,
188.8.131.52 Stop marks, or
184.108.40.206 Pipe reducer ripple.
14.8 The test methods described in this section are not
necessarily capable of inspecting the end portion of pipes, a
condition referred to as “end effect.” The length of such end
effect shall be determined by the manufacturer and, when
speciﬁed in the purchase order, reported to the purchaser.
15.1 Nipples shall be cut from pipe of the same dimensions
and quality described in this speciﬁcation.
16. Dimensions, Weight, and Permissible Variations
16.1 Weight—The weight of any length of pipe shall not
vary more than 10 % over and 3.5 % under that speciﬁed.
Unless otherwise agreed upon between the manufacturer and
the purchaser, pipe in NPS 4 and smaller may be weighed in
convenient lots; pipe larger than NPS 4 shall be weighed
16.2 Diameter—The tolerances for diameter shall be in
accordance with the following:
16.2.1 Except for pipe ordered as special outside diameter
tolerance pipe or as inside diameter tolerance pipe, variations
in outside diameter shall not exceed those precribed in Table 5.
16.2.2 For pipe over 10 in. (254 mm) OD ordered as special
outside diameter tolerance pipe, the outside diameter shall not
vary more than 1 % over or 1 % under the speciﬁed outside
16.2.3 For pipe over 10 in. (254 mm) ID ordered as inside
diameter tolerance pipe, the inside diameter shall not vary
more than 1 % over or 1 % under the speciﬁed inside diameter.
16.3 Thickness—The minimum wall thickness at any point
shall not be more than 12.5 % under the nominal wall thickness
NOTE 7—The minimum wall thicknesses on inspection of some of the
available sizes are shown in Table X2.1.
17.1 Pipe lengths shall be in accordance with the following
17.1.1 The lengths required shall be speciﬁed in the order,
17.1.2 No jointers are permitted unless otherwise speciﬁed.
17.1.3 If deﬁnite lengths are not required, pipe may be
ordered in single random lengths of 16 to 22 ft (4.8 to 6.7 m)
with 5 % 12 to 16 ft (3.7 to 4.8 m), or in double random lengths
with a minimum average of 35 ft (10.7 m) and a minimum
length of 22 ft with 5 % 16 to 22 ft.
18. Workmanship, Finish and Appearance
18.1 The pipe manufacturer shall explore a sufficient num-
ber of visual surface imperfections to provide reasonable
TABLE 5 Variations in Outside Diameter
NPS Designator Permissible Variations in Outside
in. mm in. mm
1⁄8to 11⁄2, incl 1⁄64(0.015) 0.40 1⁄64(0.015) 0.40
Over 11⁄2 to 4, incl 1⁄32 (0.031) 0.79 1⁄32 (0.031) 0.79
Over 4 to 8, incl 1⁄16(0.062) 1.59 1⁄32(0.031) 0.79
Over 8 to 18, incl 3⁄32(0.093) 2.38 1⁄32 (0.031) 0.79
Over 18 to 26, incl 1⁄8(0.125) 3.18 1⁄32 (0.031) 0.79
Over 26 to 34, incl 5⁄32(0.156) 3.97 1⁄32 (0.031) 0.79
Over 34 to 48, incl 3⁄16(0.187) 4.76 1⁄32(0.031) 0.79
assurance that they have been properly evaluated with respect
to depth. Exploration of all surface imperfections is not
required but consideration should be given to the necessity of
exploring all surface imperfections to assure compliance with
18.2 Surface imperfections that penetrate more than 121⁄2 %
of the nominal wall thickness or encroach on the minimum
wall thickness shall be considered defects. Pipe with such
defects shall be given one of the following dispositions:
18.2.1 The defect shall be removed by grinding, provided
that the remaining wall thickness is within the limits speciﬁed
18.2.2 Repaired in accordance with the repair welding
provisions of 18.6.
18.2.3 The section of pipe containing the defect may be cut
off within the limits of requirements on length.
18.3 To provide a workmanlike ﬁnish and basis for evalu-
ating conformance with 18.2 the pipe manufacturer shall
remove by grinding the following noninjurious imperfections:
18.3.1 Mechanical marks, abrasions (Note 8) and pits, any
of which imperfections are deeper than 1⁄16 in. (1.58 mm).
18.3.2 Visual imperfections commonly referred to as scabs,
seams, laps, tears, or slivers found by exploration in accor-
dance with 18.1 to be deeper than 5 % of the nominal wall
18.4 At the purchaser’s discretion, pipe shall be subjected to
rejection if surface imperfections acceptable under 18.2 are not
scattered, but appear over a large area in excess of what is
considered a workmanlike ﬁnish. Disposition of such pipe shall
be a matter of agreement between the manufacturer and the
18.5 When imperfections or defects are removed by grind-
ing, a smooth curved surface shall be maintained, and the wall
thickness shall not be decreased below that permitted by this
speciﬁcation. The outside diameter at the point of grinding is
permitted to be reduced by the amount so removed.
18.5.1 Wall thickness measurements shall be made with a
mechanical caliper or with a properly calibrated nondestructive
testing device of appropriate accuracy. In case of dispute, the
measurement determined by use of the mechanical caliper shall
18.6 Weld repair shall be permitted only subject to the
approval of the purchaser and in accordance with Speciﬁcation
A 530/A 530M.
18.7 The ﬁnished pipe shall be reasonably straight.
NOTE 8—Marks and abrasions are deﬁned as cable marks, dinges, guide
marks, roll marks, ball scratches, scores, die marks, etc.
19. End Finish
19.1 The Pipe shall be furnished to the following practice,
unless otherwise speciﬁed.
19.1.1 NPS 1-1/2 and Smaller—All walls shall be either
plain-end square cut, or plain-end beveled at the option of the
19.1.2 NPS 2 and Larger—Walls through extra strong
weights, shall be plain end-beveled.
19.1.3 NPS 2 and Larger—Walls over extra strong weights,
shall be plain-end square cut.
NOTE 9—Plain-end beveled is deﬁned as plain-end pipe having a bevel
angle of 30°, +5° or -0°, as measured from a line drawn perpendicular to
the axis of the pipe with a root face of 1⁄16 6 1⁄32in. (1.5875 6 0.7938 mm).
Other bevel angles may be speciﬁed by agreement between the purchaser
and the manufacturer.
20. Number of Tests
20.1 The tensile requirements speciﬁed in Section 7 shall be
determined on one length of pipe from each lot (Note 4) of 400
lengths or fraction thereof of each size under NPS 6, and from
each lot of 200 lengths or fraction thereof of each size NPS 6
20.2 For pipe NPS 2 and under, the bend test speciﬁed in
11.1 shall be made on one pipe from each lot of 400 lengths or
fraction thereof of each size. The bend test, where used as
permitted by 11.2 or required by 11.3, shall be made on one end
of 5 % of the pipe from each lot. For small lots, at least one
pipe shall be tested.
20.3 The ﬂattening test speciﬁed in Section 12 shall be
made on one length of pipe from each lot of 400 lengths or
fraction thereof of each size over NPS 2, up to but not
including NPS 6, and from each lot of 200 lengths or fraction
thereof, of each size NPS 6 and over.
20.4 Each length of pipe shall be subjected to the hydro-
static test speciﬁed in Section 13.
20.5 If any test specimen shows defective machining or
develops ﬂaws, it is permissible to discard the ﬂawed specimen
and substitute another specimen.
21.1 If the percentage of elongation of any tension test
specimen is less than that prescribed in Table 1 and any part of
the fracture is more than 3⁄4in. (19.0 mm) from the center of the
gage length of a 2-in. (50-mm) specimen as indicated by scribe
scratches marked on the specimen before testing, a retest shall
be allowed. If a specimen breaks in an inside or outside surface
ﬂaw, a retest shall be allowed.
21.2 Should a crop end of a ﬁnished pipe fail in the
ﬂattening test, one retest is permitted to be made from the
failed end. Pipe shall be normalized either before or after the
ﬁrst test, but pipe shall be subjected to only two normalizing
22. Test Specimens and Test Methods
22.1 On NPS 8 and larger, specimens cut either longitudi-
nally or transversely shall be acceptable for the tension test. On
sizes smaller than NPS 8, the longitudinal test only shall be
22.2 When round tension test specimens are used for pipe
wall thicknesses over 1.0 in. (25.40 mm), the mid–length of the
longitudinal axis of such test specimens shall be from a
location midway between the inside and outside surfaces of the
22.3 Test specimens for the bend test speciﬁed in Section 11
and for the ﬂattening tests shall consist of sections cut from a
pipe. Specimens for ﬂattening tests shall be smooth on the ends
and free from burrs, except when made on crop ends.
22.4 Test specimens for the bend test speciﬁed in 11.2 and
11.3 shall be cut from one end of the pipe and, unless otherwise
speciﬁed, shall be taken in a transverse direction. One test
specimen shall be taken as close to the outer surface as possible
and another from as close to the inner surface as possible. The
specimens shall be either 1⁄2 by 1⁄2 in. (12.7 by 12.7 mm) in
section or 1 by 1⁄2 in. (25.4 by 12.7 mm) in section with the
corners rounded to a radius not over 1⁄16 in. (1.6 mm) and need
not exceed 6 in. (152 mm) in length. The side of the samples
placed in tension during the bend shall be the side closest to the
inner and outer surface of the pipe respectively.
22.5 All routine check tests shall be made at room tempera-
23.1 When test reports are requested, in addition to the
requirements of Speciﬁcation A 530/A 530M, the producer or
supplier shall furnish to the purchaser a chemical analysis
report for the elements speciﬁed in Table 1.
24. Product Marking
24.1 In addition to the marking prescribed in Speciﬁcation
A 530/A 530M, the marking shall include heat number, the
information as per Table 6, an additional symbol“ S” if one or
more of the supplementary requirements apply; the length, OD
1 %, if ordered as special outside diameter tolerance pipe; ID
1 %, if ordered as special inside diameter tolerance pipe; the
schedule number, weight class, or nominal wall thickness; and,
for sizes larger than NPS 4, the weight. Length shall be marked
in feet and tenths of a foot, or metres to two decimal places,
depending on the units to which the material was ordered, or
other marking subject to agreement. For sizes NPS 11⁄2, 11⁄4, 1,
and 3⁄4, each length shall be marked as prescribed in Speciﬁ-
cation A 530/A 530M. These sizes shall be bundled in accor-
dance with standard mill practice and the total bundle footage
marked on the bundle tag; individual lengths of pipe need not
be marked with footage. For sizes less than NPS 3⁄4, all the
required markings shall be on the bundle tag or on each length
of pipe and shall include the total footage; individual lengths of
pipe need not be marked with footage. If not marked on the
bundle tag, all required marking shall be on each length.
24.2 When pipe sections are cut into shorter lengths by a
subsequent processor for resale as material, the processor shall
transfer complete identifying information, including the name
or brand of the manufacturer to each unmarked cut length, or
to metal tags securely attached to bundles of unmarked small
diameter pipe. The same material designation shall be included
with the information transferred, and the processor’s name,
trademark, or brand shall be added.
24.3 Bar Coding—In addition to the requirements in 24.1
and 24.2, bar coding is acceptable as a supplementary identi-
ﬁcation method. The purchaser may specify in the order a
speciﬁc bar coding system to be used.
25. Government Procurement
25.1 When speciﬁed in the contract, material shall be
preserved, packaged, and packed in accordance with the
requirements of MIL-STD-163. The applicable levels shall be
as speciﬁed in the contract. Marking for the shipment of such
material shall be in accordance with Fed. Std. No. 123 for civil
agencies and MIL-STD-129 or Fed. Std. No. 183 if continuous
marking is required for military agencies.
25.2 Inspection—Unless otherwise speciﬁed in the contract,
the producer is responsible for the performance of all inspec-
tion and test requirements speciﬁed herein. Except as otherwise
speciﬁed in the contract, the producer shall use his own, or any
other suitable facilities for the performance of the inspection
and test requirements speciﬁed herein, unless disapproved by
the purchaser. The purchaser shall have the right to perform
any of the inspections and tests set forth in this speciﬁcation
where such inspections are deemed necessary to ensure that the
material conforms to the prescribed requirements.
26.1 carbon steel pipe; seamless steel pipe; steel pipe
One or more of the following supplementary requirements shall apply only when speciﬁed in the
purchase order. The purchaser may specify a different frequency of test or analysis than is provided
in the supplementary requirement. Subject to agreement between the purchaser and manufacturer,
retest and retreatment provisions of these supplementary requirements may also be modiﬁed.
S1. Product Analysis
S1.1 Product analysis shall be made on each length of pipe.
Individual lengths failing to conform to the chemical compo-
sition requirements shall be rejected.
S2. Transverse Tension Test
S2.1 A transverse tension test shall be made on a specimen
from one end or both ends of each pipe NPS 8 and over. If this
supplementary requirement is speciﬁed, the number of tests per
pipe shall also be speciﬁed. If a specimen from any length fails
to meet the required tensile properties (tensile, yield, and
elongation), that length shall be rejected subject to retreatment
in accordance with Speciﬁcation A 530/A 530M and satisfac-
TABLE 6 Marking
Hydro NDE Marking
Yes No Test Pressure
No Yes NDE
No No NH
Yes Yes Test Pressure/NDE
S3. Flattening Test
S3.1 The ﬂattening test of Speciﬁcation A 530/A 530M
shall be made on a specimen from one end or both ends of each
pipe. Crop ends may be used. If this supplementary require-
ment is speciﬁed, the number of tests per pipe shall also be
speciﬁed. If a specimen from any length fails because of lack
of ductility prior to satisfactory completion of the ﬁrst step of
the ﬂattening test requirement, that pipe shall be rejected
subject to retreatment in accordance with Speciﬁcation A 530/
A 530M and satisfactory retest. If a specimen from any length
of pipe fails because of a lack of soundness, that length shall be
rejected, unless subsequent retesting indicates that the remain-
ing length is sound.
S4. Metal Structure and Etching Test
S4.1 The steel shall be homogeneous as shown by etching
tests conducted in accordance with the appropriate sections of
Method E 381. Etching tests shall be made on a cross section
from one end or both ends of each pipe and shall show sound
and reasonably uniform material free from injurious lamina-
tions, cracks, and similar objectionable defects. If this supple-
mentary requirement is speciﬁed, the number of tests per pipe
required shall also be speciﬁed. If a specimen from any length
shows objectionable defects, the length shall be rejected,
subject to removal of the defective end and subsequent retests
indicating the remainder of the length to be sound and
reasonably uniform material.
S5. Carbon Equivalent
S5.1 The steel shall conform to a carbon equivalent (CE) of
0.50 maximum as determined by the following formula:
CE 5 %C 1
%Cr 1 %Mo 1 %V
%Ni 1 %Cu
S5.2 A lower CE maximum may be agreed upon between
the purchaser and the producer.
S5.3 The CE shall be reported on the test report.
S6. Heat Treated Test Specimens
S6.1 At the request of the purchaser, one tensile test shall be
performed by the manufacturer on a test specimen from each
heat of steel furnished which has been either stress relieved at
1250°F or normalized at 1650°F, as speciﬁed by the purchaser.
Other stress relief or annealing temperatures, as appropriate to
the analysis, may be speciﬁed by agreement between the
purchaser and the manufacturer. The results of this test shall
meet the requirements of Table 1.
S7. Internal Cleanliness–Government Orders
S7.1 The internal surface of hot ﬁnished ferritic steel pipe
and tube shall be manufactured to a free of scale condition
equivalent to the visual standard listed in SSPC-SP6. Cleaning
shall be performed in accordance with a written procedure that
has been shown to be effective. This procedure shall be
available for audit.
X1. CALCULATED H VALUES FOR SEAMLESS PIPE
X1.1 Tables X1.1 and X1.2 list values for H to be used for
the test of Section 12.
X2. MINIMUM WALL THICKNESS
X2.1 Table X2.1 lists minimum wall thicknesses for nomi- nal pipe wall thickness.
The American Society for Testing and Materials takes no position respecting the validity of any patent rights asserted in connection
with any item mentioned in this standard. Users of this standard are expressly advised that determination of the validity of any such
patent rights, and the risk of infringement of such rights, are entirely their own responsibility.
This standard is subject to revision at any time by the responsible technical committee and must be reviewed every ﬁve years and
if not revised, either reapproved or withdrawn. Your comments are invited either for revision of this standard or for additional standards
and should be addressed to ASTM Headquarters. Your comments will receive careful consideration at a meeting of the responsible
technical committee, which you may attend. If you feel that your comments have not received a fair hearing you should make your
views known to the ASTM Committee on Standards, at the address shown below.
TABLE X2.1 Mimimum Wall Thicknesses on Inspection for Nominal (Average) Pipe Wall Thicknesses
NOTE 1—The following equation, upon which this table is based, may be applied to calculate minimum wall thickness from nominal (average) wall
tn 3 0.875 5 tm
tn = nominal (average) wall thickness, in. and
tm = minimum wall thickness, in.
The wall thickness is expressed to three decimal places, the fourth decimal place being carried forward or dropped, in accordance with Practice E 29.
NOTE 2—This table covers some wall thicknesses associated with standard pipe sizes but is not meant to imply that these are the only thicknesses
obtainable under this speciﬁcation.
in. mm in. mm in. mm in. mm in. mm in. mm
0.068 1.73 0.060 1.52 0.281 7.14 0.246 6.25 0.864 21.94 0.756 19.20
0.083 2.11 0.073 1.85 0.294 7.47 0.257 6.53 0.875 22.22 0.766 19.46
0.088 2.24 0.077 1.96 0.300 7.62 0.262 6.65 0.906 23.01 0.793 20.14
0.091 2.31 0.080 2.03 0.307 7.80 0.269 6.83 0.938 23.82 0.821 20.85
0.095 2.41 0.083 2.11 0.308 7.82 0.270 6.86 0.968 24.59 0.847 21.51
0.109 2.77 0.095 2.41 0.312 7.92 0.273 6.93 1.000 25.40 0.875 22.22
0.113 2.87 0.099 2.51 0.318 8.07 0.278 7.06 1.031 26.19 0.902 22.91
0.119 3.02 0.104 2.64 0.322 8.18 0.282 7.16 1.062 26.97 0.929 23.60
0.125 3.18 0.109 2.77 0.330 8.38 0.289 7.34 1.094 27.79 0.957 24.31
0.126 3.20 0.110 2.79 0.337 8.56 0.295 7.49 1.125 28.58 0.984 24.99
0.133 3.38 0.116 2.95 0.344 8.74 0.301 7.64 1.156 29.36 1.012 25.70
0.140 3.56 0.122 3.10 0.358 9.09 0.313 7.95 1.219 30.96 1.066 27.08
0.141 3.58 0.123 3.12 0.365 9.27 0.319 8.10 1.250 31.75 1.094 27.79
0.145 3.68 0.127 3.23 0.375 9.52 0.328 8.33 1.281 32.54 1.121 28.47
0.147 3.73 0.129 3.28 0.382 9.70 0.334 8.48 1.312 33.32 1.148 29.16
0.154 3.91 0.135 3.43 0.400 10.16 0.350 8.89 1.375 34.92 1.203 30.56
0.156 3.96 0.136 3.45 0.406 10.31 0.355 9.02 1.406 35.71 1.230 31.24
0.172 4.37 0.150 3.81 0.432 10.97 0.378 9.60 1.438 36.53 1.258 31.95
0.179 4.55 0.157 3.99 0.436 11.07 0.382 9.70 1.500 38.10 1.312 33.32
0.188 4.78 0.164 4.17 0.438 11.12 0.383 9.73 1.531 38.89 1.340 34.04
0.191 4.85 0.167 4.24 0.469 11.91 0.410 10.41 1.562 39.67 1.367 34.72
0.200 5.08 0.175 4.44 0.500 12.70 0.438 11.13 1.594 40.49 1.395 35.43
0.203 5.16 0.178 4.52 0.531 13.49 0.465 11.81 1.635 41.53 1.431 36.35
0.210 5.33 0.184 4.67 0.552 14.02 0.483 12.27 1.750 44.45 1.531 38.89
0.216 5.49 0.189 4.80 0.562 14.27 0.492 12.50 1.781 45.24 1.558 39.57
0.218 5.54 0.191 4.85 0.594 15.09 0.520 13.21 1.812 46.02 1.586 40.28
0.219 5.56 0.192 4.88 0.600 15.24 0.525 13.34 1.875 47.62 1.641 41.68
0.226 5.74 0.198 5.03 0.625 15.88 0.547 13.89 1.969 50.01 1.723 43.76
0.237 6.02 0.207 5.26 0.656 16.66 0.574 14.58 2.000 50.80 1.750 44.45
0.250 6.35 0.219 5.56 0.674 17.12 0.590 14.99 2.062 52.37 1.804 45.82
0.258 6.55 0.226 5.74 0.688 17.48 0.602 15.29 2.125 53.98 1.859 47.22
0.276 7.01 0.242 6.15 0.719 18.26 0.629 15.98 2.200 55.88 1.925 48.90
0.277 7.04 0.242 6.15 0.750 19.05 0.656 16.66 2.344 59.54 2.051 52.10
0.279 7.09 0.244 6.19 0.812 20.62 0.710 18.03 2.500 63.50 2.188 55.58
0.280 7.11 0.245 6.22 0.844 21.44 0.739 18.77
This standard is copyrighted by ASTM, 100 Barr Harbor Drive, PO Box C700, West Conshohocken, PA 19428-2959, United States.
Individual reprints (single or multiple copies) of this standard may be obtained by contacting ASTM at the above address or at
610-832-9585 (phone), 610-832-9555 (fax), or firstname.lastname@example.org (e-mail); or through the ASTM website (www.astm.org).